#------------------------------------------------------------------------------
#$Date: 2016-03-23 23:57:12 +0200 (Wed, 23 Mar 2016) $
#$Revision: 179519 $
#$URL: svn://www.crystallography.net/cod/cif/4/34/16/4341662.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4341662
loop_
_publ_author_name
'Treadwell, LaRico J'
'Watkins-Curry, Pilanda'
'McAlpin, Jacob D.'
'Rebar, Drew J.'
'Hebert, Jessica K.'
'DiTusa, John F.'
'Chan, Julia Y.'
_publ_section_title
;
 Investigation of Mn, Fe, and Ni Incorporation in CeCo2Al8.
;
_journal_issue                   3
_journal_name_full               'Inorganic chemistry'
_journal_page_first              963
_journal_page_last               968
_journal_paper_doi               10.1021/ic502356t
_journal_volume                  54
_journal_year                    2015
_chemical_formula_moiety         'Al8 Ce Co1.71 Ni0.27'
_chemical_formula_sum            'Al8 Ce Co1.71 Ni0.27'
_chemical_formula_weight         473.60
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           55
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-P 2 2ab'
_symmetry_space_group_name_H-M   'P b a m'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_audit_update_record
;
2014-10-27 # Formatted by publCIF
;
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   12.4770(10)
_cell_length_b                   14.393(4)
_cell_length_c                   4.023(4)
_cell_measurement_temperature    293(2)
_cell_volume                     722.5(7)
_computing_cell_refinement       'Denzo and Scalepack (Otwinski & Minor 1997)'
_computing_data_collection       'Collect (Nonius 1999)'
_computing_data_reduction        'Denzo and Scalepack (Otwinski & Minor 1997)'
_computing_molecular_graphics    'Crystal Maker'
_computing_publication_material  Publcif
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.989
_diffrn_measured_fraction_theta_max 0.989
_diffrn_measurement_device_type  'Nonius Kappa CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0488
_diffrn_reflns_av_sigmaI/netI    0.0556
_diffrn_reflns_limit_h_max       18
_diffrn_reflns_limit_h_min       -17
_diffrn_reflns_limit_k_max       20
_diffrn_reflns_limit_k_min       -20
_diffrn_reflns_limit_l_max       5
_diffrn_reflns_limit_l_min       -5
_diffrn_reflns_number            2148
_diffrn_reflns_theta_full        31.19
_diffrn_reflns_theta_max         31.19
_diffrn_reflns_theta_min         3.27
_exptl_absorpt_coefficient_mu    11.910
_exptl_absorpt_correction_T_max  0.700
_exptl_absorpt_correction_T_min  0.658
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'HKL scalepack (Otwinski & Minor, 1997)'
_exptl_crystal_colour            silver
_exptl_crystal_density_diffrn    4.354
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       Fragment
_exptl_crystal_F_000             868
_exptl_crystal_size_max          0.04
_exptl_crystal_size_mid          0.03
_exptl_crystal_size_min          0.03
_refine_diff_density_max         1.441
_refine_diff_density_min         -1.559
_refine_diff_density_rms         0.313
_refine_ls_extinction_coef       0.0023(2)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.032
_refine_ls_matrix_type           full
_refine_ls_number_parameters     72
_refine_ls_number_reflns         1302
_refine_ls_number_restraints     1
_refine_ls_restrained_S_all      1.032
_refine_ls_R_factor_all          0.0645
_refine_ls_R_factor_gt           0.0367
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0288P)²+1.9393P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0702
_refine_ls_wR_factor_ref         0.0805
_reflns_number_gt                942
_reflns_number_total             1302
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic502356t_si_009.cif
_cod_data_source_block           shelx
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Orthorhombic' changed to
'orthorhombic' according to
/home/saulius/struct/COD-crude-data--automatic-downloads/rss-feeds/ACS/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from
2011-04-26.

'_exptl_absorpt_correction_type' value 'Multi-scan'
changed to 'multi-scan' according to
/home/saulius/struct/COD-crude-data--automatic-downloads/rss-feeds/ACS/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 2935 2014-11-11 08:27:57Z andrius 

 Adding full bibliography for 4341656--4341665.cif.
;
_cod_original_sg_symbol_H-M      Pbam
_cod_database_code               4341662
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, z'
'x+1/2, -y+1/2, -z'
'-x+1/2, y+1/2, -z'
'-x, -y, -z'
'x, y, -z'
'-x-1/2, y-1/2, z'
'x-1/2, -y-1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Ce1 Ce 0.34045(4) 0.31846(3) 0.0000 0.01140(14) Uani 1 2 d S
Ni1 Ni 0.03474(8) 0.40566(7) 0.0000 0.0096(3) Uani 0.270(2) 2 d SP
Co1 Co 0.03474(8) 0.40566(7) 0.0000 0.0096(3) Uani 0.712(5) 2 d SP
Co2 Co 0.15175(8) 0.09647(7) 0.0000 0.0084(2) Uani 1 2 d S
Al1 Al 0.02525(19) 0.13187(15) 0.5000 0.0101(5) Uani 1 2 d S
Al2 Al 0.1597(2) 0.37941(16) 0.5000 0.0104(4) Uani 1 2 d S
Al3 Al 0.23657(19) 0.17249(16) 0.5000 0.0107(5) Uani 1 2 d S
Al4 Al 0.3318(2) 0.49153(15) 0.5000 0.0103(5) Uani 1 2 d S
Al5 Al 0.45226(18) 0.17961(16) 0.5000 0.0108(5) Uani 1 2 d S
Al6 Al 0.0961(2) 0.25283(16) 0.0000 0.0108(4) Uani 1 2 d S
Al7 Al 0.3399(2) 0.04440(16) 0.0000 0.0116(5) Uani 1 2 d S
Al8 Al 0.0000 0.5000 0.5000 0.0101(7) Uani 1 4 d S
Al9 Al 0.0000 0.0000 0.0000 0.0111(7) Uani 1 4 d S
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Ce Ce -0.2486 2.6331 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Co Co 0.3494 0.9721 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ni Ni 0.3393 1.1124 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Al Al 0.0645 0.0514 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
Al1 Ce1 Al1 79.60(8) 3_556 3
Al1 Ce1 Al2 150.65(6) 3_556 1_554
Al1 Ce1 Al2 93.05(7) 3 1_554
Al1 Ce1 Al2 93.06(7) 3_556 .
Al1 Ce1 Al2 150.66(6) 3 .
Al2 Ce1 Al2 79.47(8) 1_554 .
Al1 Ce1 Al5 103.14(7) 3_556 1_554
Al1 Ce1 Al5 54.02(6) 3 1_554
Al2 Ce1 Al5 94.92(7) 1_554 1_554
Al2 Ce1 Al5 154.11(6) . 1_554
Al1 Ce1 Al5 54.02(6) 3_556 .
Al1 Ce1 Al5 103.14(7) 3 .
Al2 Ce1 Al5 154.11(6) 1_554 .
Al2 Ce1 Al5 94.92(7) . .
Al5 Ce1 Al5 79.07(8) 1_554 .
Al1 Ce1 Al3 148.55(6) 3_556 1_554
Al1 Ce1 Al3 92.54(7) 3 1_554
Al2 Ce1 Al3 59.23(6) 1_554 1_554
Al2 Ce1 Al3 107.22(7) . 1_554
Al5 Ce1 Al3 50.23(6) 1_554 1_554
Al5 Ce1 Al3 99.47(6) . 1_554
Al1 Ce1 Al3 92.54(7) 3_556 .
Al1 Ce1 Al3 148.55(6) 3 .
Al2 Ce1 Al3 107.22(7) 1_554 .
Al2 Ce1 Al3 59.23(6) . .
Al5 Ce1 Al3 99.47(6) 1_554 .
Al5 Ce1 Al3 50.23(6) . .
Al3 Ce1 Al3 78.35(8) 1_554 .
Al1 Ce1 Al6 140.20(4) 3_556 .
Al1 Ce1 Al6 140.20(4) 3 .
Al2 Ce1 Al6 52.98(5) 1_554 .
Al2 Ce1 Al6 52.98(5) . .
Al5 Ce1 Al6 103.56(5) 1_554 .
Al5 Ce1 Al6 103.56(5) . .
Al3 Ce1 Al6 54.26(5) 1_554 .
Al3 Ce1 Al6 54.26(5) . .
Al1 Ce1 Al4 104.46(6) 3_556 1_554
Al1 Ce1 Al4 56.35(6) 3 1_554
Al2 Ce1 Al4 50.04(6) 1_554 1_554
Al2 Ce1 Al4 99.23(7) . 1_554
Al5 Ce1 Al4 96.14(7) 1_554 1_554
Al5 Ce1 Al4 155.00(7) . 1_554
Al3 Ce1 Al4 95.89(7) 1_554 1_554
Al3 Ce1 Al4 153.63(7) . 1_554
Al6 Ce1 Al4 101.42(6) . 1_554
Al1 Ce1 Al4 56.35(6) 3_556 .
Al1 Ce1 Al4 104.46(6) 3 .
Al2 Ce1 Al4 99.23(7) 1_554 .
Al2 Ce1 Al4 50.04(6) . .
Al5 Ce1 Al4 155.00(7) 1_554 .
Al5 Ce1 Al4 96.14(7) . .
Al3 Ce1 Al4 153.63(7) 1_554 .
Al3 Ce1 Al4 95.89(7) . .
Al6 Ce1 Al4 101.42(6) . .
Al4 Ce1 Al4 77.79(8) 1_554 .
Al1 Ce1 Al9 51.27(4) 3_556 3
Al1 Ce1 Al9 51.27(4) 3 3
Al2 Ce1 Al9 102.27(4) 1_554 3
Al2 Ce1 Al9 102.28(4) . 3
Al5 Ce1 Al9 103.62(5) 1_554 3
Al5 Ce1 Al9 103.62(5) . 3
Al3 Ce1 Al9 140.49(4) 1_554 3
Al3 Ce1 Al9 140.49(4) . 3
Al6 Ce1 Al9 144.52(4) . 3
Al4 Ce1 Al9 53.27(4) 1_554 3
Al4 Ce1 Al9 53.27(4) . 3
Al6 Ni1 Al8 125.31(3) . .
Al6 Ni1 Al8 125.31(3) . 1_554
Al8 Ni1 Al8 109.36(7) . 1_554
Al6 Ni1 Al7 122.72(10) . 7_665
Al8 Ni1 Al7 71.03(4) . 7_665
Al8 Ni1 Al7 71.03(4) 1_554 7_665
Al6 Ni1 Al7 125.67(9) . 3_455
Al8 Ni1 Al7 71.05(4) . 3_455
Al8 Ni1 Al7 71.05(4) 1_554 3_455
Al7 Ni1 Al7 111.61(7) 7_665 3_455
Al6 Ni1 Al5 71.39(7) . 3_455
Al8 Ni1 Al5 146.18(7) . 3_455
Al8 Ni1 Al5 63.53(6) 1_554 3_455
Al7 Ni1 Al5 128.50(5) 7_665 3_455
Al7 Ni1 Al5 75.61(7) 3_455 3_455
Al6 Ni1 Al5 71.39(7) . 3_456
Al8 Ni1 Al5 63.53(6) . 3_456
Al8 Ni1 Al5 146.18(7) 1_554 3_456
Al7 Ni1 Al5 128.50(5) 7_665 3_456
Al7 Ni1 Al5 75.61(7) 3_455 3_456
Al5 Ni1 Al5 102.94(10) 3_455 3_456
Al6 Ni1 Al2 70.25(7) . .
Al8 Ni1 Al2 63.22(6) . .
Al8 Ni1 Al2 145.62(7) 1_554 .
Al7 Ni1 Al2 75.04(7) 7_665 .
Al7 Ni1 Al2 128.51(5) 3_455 .
Al5 Ni1 Al2 141.63(8) 3_455 .
Al5 Ni1 Al2 63.95(8) 3_456 .
Al6 Ni1 Al2 70.25(7) . 1_554
Al8 Ni1 Al2 145.62(7) . 1_554
Al8 Ni1 Al2 63.22(6) 1_554 1_554
Al7 Ni1 Al2 75.04(7) 7_665 1_554
Al7 Ni1 Al2 128.51(5) 3_455 1_554
Al5 Ni1 Al2 63.95(8) 3_455 1_554
Al5 Ni1 Al2 141.63(8) 3_456 1_554
Al2 Ni1 Al2 102.86(11) . 1_554
Al6 Ni1 Co1 178.50(9) . 5_565
Al8 Ni1 Co1 54.68(3) . 5_565
Al8 Ni1 Co1 54.68(3) 1_554 5_565
Al7 Ni1 Co1 55.78(7) 7_665 5_565
Al7 Ni1 Co1 55.83(6) 3_455 5_565
Al5 Ni1 Co1 109.45(6) 3_455 5_565
Al5 Ni1 Co1 109.45(6) 3_456 5_565
Al2 Ni1 Co1 108.92(6) . 5_565
Al2 Ni1 Co1 108.92(6) 1_554 5_565
Al6 Ni1 Ni1 178.50(9) . 5_565
Al8 Ni1 Ni1 54.68(3) . 5_565
Al8 Ni1 Ni1 54.68(3) 1_554 5_565
Al7 Ni1 Ni1 55.78(7) 7_665 5_565
Al7 Ni1 Ni1 55.83(6) 3_455 5_565
Al5 Ni1 Ni1 109.45(6) 3_455 5_565
Al5 Ni1 Ni1 109.45(6) 3_456 5_565
Al2 Ni1 Ni1 108.92(6) . 5_565
Al2 Ni1 Ni1 108.92(6) 1_554 5_565
Co1 Ni1 Ni1 0.00(4) 5_565 5_565
Al9 Co2 Al6 109.12(7) . .
Al9 Co2 Al7 126.04(7) . .
Al6 Co2 Al7 124.84(9) . .
Al9 Co2 Al3 126.50(5) . .
Al6 Co2 Al3 73.09(7) . .
Al7 Co2 Al3 74.47(7) . .
Al9 Co2 Al3 126.50(6) . 1_554
Al6 Co2 Al3 73.09(7) . 1_554
Al7 Co2 Al3 74.47(7) . 1_554
Al3 Co2 Al3 105.77(11) . 1_554
Al9 Co2 Al4 73.24(6) . 7_654
Al6 Co2 Al4 126.58(5) . 7_654
Al7 Co2 Al4 74.96(7) . 7_654
Al3 Co2 Al4 149.43(9) . 7_654
Al3 Co2 Al4 65.79(8) 1_554 7_654
Al9 Co2 Al4 73.24(6) . 7_655
Al6 Co2 Al4 126.58(5) . 7_655
Al7 Co2 Al4 74.96(7) . 7_655
Al3 Co2 Al4 65.79(8) . 7_655
Al3 Co2 Al4 149.43(9) 1_554 7_655
Al4 Co2 Al4 105.69(10) 7_654 7_655
Al9 Co2 Al1 68.12(6) . 1_554
Al6 Co2 Al1 68.59(6) . 1_554
Al7 Co2 Al1 129.51(5) . 1_554
Al3 Co2 Al1 141.67(8) . 1_554
Al3 Co2 Al1 63.51(8) 1_554 1_554
Al4 Co2 Al1 63.34(8) 7_654 1_554
Al4 Co2 Al1 141.36(9) 7_655 1_554
Al9 Co2 Al1 68.12(6) . .
Al6 Co2 Al1 68.59(6) . .
Al7 Co2 Al1 129.51(5) . .
Al3 Co2 Al1 63.51(8) . .
Al3 Co2 Al1 141.67(8) 1_554 .
Al4 Co2 Al1 141.36(9) 7_654 .
Al4 Co2 Al1 63.34(8) 7_655 .
Al1 Co2 Al1 100.99(10) 1_554 .
Co2 Al1 Co2 100.99(11) . 1_556
Co2 Al1 Al4 56.82(6) . 7_655
Co2 Al1 Al4 56.82(6) 1_556 7_655
Co2 Al1 Al3 56.72(6) . .
Co2 Al1 Al3 56.72(6) 1_556 .
Al4 Al1 Al3 61.06(9) 7_655 .
Co2 Al1 Al9 51.52(4) . .
Co2 Al1 Al9 119.53(9) 1_556 .
Al4 Al1 Al9 64.14(6) 7_655 .
Al3 Al1 Al9 104.96(7) . .
Co2 Al1 Al9 119.53(9) . 1_556
Co2 Al1 Al9 51.52(4) 1_556 1_556
Al4 Al1 Al9 64.14(6) 7_655 1_556
Al3 Al1 Al9 104.96(7) . 1_556
Al9 Al1 Al9 92.55(9) . 1_556
Co2 Al1 Al6 51.45(6) . .
Co2 Al1 Al6 118.94(10) 1_556 .
Al4 Al1 Al6 104.87(9) 7_655 .
Al3 Al1 Al6 63.74(7) . .
Al9 Al1 Al6 86.60(7) . .
Al9 Al1 Al6 167.87(11) 1_556 .
Co2 Al1 Al6 118.94(10) . 1_556
Co2 Al1 Al6 51.45(6) 1_556 1_556
Al4 Al1 Al6 104.87(9) 7_655 1_556
Al3 Al1 Al6 63.74(7) . 1_556
Al9 Al1 Al6 167.87(11) . 1_556
Al9 Al1 Al6 86.60(7) 1_556 1_556
Al6 Al1 Al6 91.69(11) . 1_556
Co2 Al1 Al5 112.20(7) . 3_456
Co2 Al1 Al5 112.20(7) 1_556 3_456
Al4 Al1 Al5 157.11(12) 7_655 3_456
Al3 Al1 Al5 96.05(10) . 3_456
Al9 Al1 Al5 127.62(6) . 3_456
Al9 Al1 Al5 127.62(6) 1_556 3_456
Al6 Al1 Al5 60.77(7) . 3_456
Al6 Al1 Al5 60.77(7) 1_556 3_456
Co2 Al1 Al4 111.83(7) . 3_456
Co2 Al1 Al4 111.83(7) 1_556 3_456
Al4 Al1 Al4 95.10(10) 7_655 3_456
Al3 Al1 Al4 156.16(11) . 3_456
Al9 Al1 Al4 60.31(5) . 3_456
Al9 Al1 Al4 60.31(5) 1_556 3_456
Al6 Al1 Al4 128.48(7) . 3_456
Al6 Al1 Al4 128.48(7) 1_556 3_456
Al5 Al1 Al4 107.79(10) 3_456 3_456
Co2 Al1 Ce1 89.70(6) . 3_455
Co2 Al1 Ce1 169.30(7) 1_556 3_455
Al4 Al1 Ce1 131.01(6) 7_655 3_455
Al3 Al1 Ce1 131.85(6) . 3_455
Al9 Al1 Ce1 67.01(5) . 3_455
Al9 Al1 Ce1 122.32(9) 1_556 3_455
Al6 Al1 Ce1 68.34(6) . 3_455
Al6 Al1 Ce1 123.33(9) 1_556 3_455
Al5 Al1 Ce1 63.31(5) 3_456 3_455
Al4 Al1 Ce1 62.86(5) 3_456 3_455
Co2 Al1 Ce1 169.30(7) . 3_456
Co2 Al1 Ce1 89.70(6) 1_556 3_456
Al4 Al1 Ce1 131.01(6) 7_655 3_456
Al3 Al1 Ce1 131.85(6) . 3_456
Al9 Al1 Ce1 122.32(9) . 3_456
Al9 Al1 Ce1 67.01(5) 1_556 3_456
Al6 Al1 Ce1 123.33(9) . 3_456
Al6 Al1 Ce1 68.34(6) 1_556 3_456
Al5 Al1 Ce1 63.31(5) 3_456 3_456
Al4 Al1 Ce1 62.86(5) 3_456 3_456
Ce1 Al1 Ce1 79.60(8) 3_455 3_456
Co1 Al2 Ni1 0.00(6) 1_556 1_556
Co1 Al2 Ni1 102.86(11) 1_556 .
Ni1 Al2 Ni1 102.86(11) 1_556 .
Co1 Al2 Al8 56.40(5) 1_556 .
Ni1 Al2 Al8 56.40(5) 1_556 .
Ni1 Al2 Al8 56.40(5) . .
Co1 Al2 Al4 113.34(7) 1_556 .
Ni1 Al2 Al4 113.34(7) 1_556 .
Ni1 Al2 Al4 113.34(7) . .
Al8 Al2 Al4 102.02(9) . .
Co1 Al2 Al5 58.00(6) 1_556 3_456
Ni1 Al2 Al5 58.00(6) 1_556 3_456
Ni1 Al2 Al5 58.00(6) . 3_456
Al8 Al2 Al5 59.23(7) . 3_456
Al4 Al2 Al5 161.25(12) . 3_456
Co1 Al2 Al6 50.84(6) 1_556 1_556
Ni1 Al2 Al6 50.84(6) 1_556 1_556
Ni1 Al2 Al6 118.75(11) . 1_556
Al8 Al2 Al6 102.23(8) . 1_556
Al4 Al2 Al6 127.68(7) . 1_556
Al5 Al2 Al6 62.14(7) 3_456 1_556
Co1 Al2 Al6 118.75(11) 1_556 .
Ni1 Al2 Al6 118.75(11) 1_556 .
Ni1 Al2 Al6 50.84(6) . .
Al8 Al2 Al6 102.23(8) . .
Al4 Al2 Al6 127.68(7) . .
Al5 Al2 Al6 62.13(7) 3_456 .
Al6 Al2 Al6 90.71(11) 1_556 .
Co1 Al2 Ce1 88.59(6) 1_556 1_556
Ni1 Al2 Ce1 88.59(6) 1_556 1_556
Ni1 Al2 Ce1 167.16(8) . 1_556
Al8 Al2 Ce1 136.35(5) . 1_556
Al4 Al2 Ce1 66.08(6) . 1_556
Al5 Al2 Ce1 126.44(7) 3_456 1_556
Al6 Al2 Ce1 64.31(6) 1_556 1_556
Al6 Al2 Ce1 118.43(10) . 1_556
Co1 Al2 Ce1 167.16(8) 1_556 .
Ni1 Al2 Ce1 167.16(8) 1_556 .
Ni1 Al2 Ce1 88.59(6) . .
Al8 Al2 Ce1 136.35(5) . .
Al4 Al2 Ce1 66.08(6) . .
Al5 Al2 Ce1 126.44(7) 3_456 .
Al6 Al2 Ce1 118.43(9) 1_556 .
Al6 Al2 Ce1 64.31(6) . .
Ce1 Al2 Ce1 79.47(8) 1_556 .
Co2 Al3 Co2 105.77(11) 1_556 .
Co2 Al3 Al5 115.83(7) 1_556 .
Co2 Al3 Al5 115.83(7) . .
Co2 Al3 Al1 59.77(6) 1_556 .
Co2 Al3 Al1 59.77(6) . .
Al5 Al3 Al1 169.68(12) . .
Co2 Al3 Al4 57.13(6) 1_556 7_655
Co2 Al3 Al4 57.13(6) . 7_655
Al5 Al3 Al4 110.31(11) . 7_655
Al1 Al3 Al4 59.36(9) . 7_655
Co2 Al3 Al6 50.80(6) 1_556 1_556
Co2 Al3 Al6 118.12(11) . 1_556
Al5 Al3 Al6 125.95(8) . 1_556
Al1 Al3 Al6 59.85(7) . 1_556
Al4 Al3 Al6 100.98(9) 7_655 1_556
Co2 Al3 Al6 118.12(11) 1_556 .
Co2 Al3 Al6 50.80(6) . .
Al5 Al3 Al6 125.95(8) . .
Al1 Al3 Al6 59.85(7) . .
Al4 Al3 Al6 100.98(9) 7_655 .
Al6 Al3 Al6 87.55(11) 1_556 .
Co2 Al3 Ce1 87.32(6) 1_556 1_556
Co2 Al3 Ce1 163.87(8) . 1_556
Al5 Al3 Ce1 64.42(6) . 1_556
Al1 Al3 Ce1 122.70(7) . 1_556
Al4 Al3 Ce1 138.91(5) 7_655 1_556
Al6 Al3 Ce1 62.99(6) 1_556 1_556
Al6 Al3 Ce1 114.83(9) . 1_556
Co2 Al3 Ce1 163.87(8) 1_556 .
Co2 Al3 Ce1 87.32(6) . .
Al5 Al3 Ce1 64.42(6) . .
Al1 Al3 Ce1 122.70(7) . .
Al4 Al3 Ce1 138.91(5) 7_655 .
Al6 Al3 Ce1 114.83(9) 1_556 .
Al6 Al3 Ce1 62.99(6) . .
Ce1 Al3 Ce1 78.35(8) 1_556 .
Co2 Al4 Co2 105.69(10) 7_666 7_665
Co2 Al4 Al2 115.12(8) 7_666 .
Co2 Al4 Al2 115.12(8) 7_665 .
Co2 Al4 Al1 59.84(6) 7_666 7_665
Co2 Al4 Al1 59.84(6) 7_665 7_665
Al2 Al4 Al1 168.37(12) . 7_665
Co2 Al4 Al3 57.08(6) 7_666 7_665
Co2 Al4 Al3 57.08(6) 7_665 7_665
Al2 Al4 Al3 108.79(11) . 7_665
Al1 Al4 Al3 59.58(8) 7_665 7_665
Co2 Al4 Al9 50.60(5) 7_666 3_556
Co2 Al4 Al9 117.86(10) 7_665 3_556
Al2 Al4 Al9 127.00(6) . 3_556
Al1 Al4 Al9 59.41(6) 7_665 3_556
Al3 Al4 Al9 100.64(7) 7_665 3_556
Co2 Al4 Al9 117.86(10) 7_666 3
Co2 Al4 Al9 50.60(5) 7_665 3
Al2 Al4 Al9 127.00(6) . 3
Al1 Al4 Al9 59.41(6) 7_665 3
Al3 Al4 Al9 100.64(7) 7_665 3
Al9 Al4 Al9 87.47(9) 3_556 3
Co2 Al4 Al1 106.81(8) 7_666 3_556
Co2 Al4 Al1 106.81(8) 7_665 3_556
Al2 Al4 Al1 106.73(10) . 3_556
Al1 Al4 Al1 84.90(10) 7_665 3_556
Al3 Al4 Al1 144.48(12) 7_665 3_556
Al9 Al4 Al1 56.21(5) 3_556 3_556
Al9 Al4 Al1 56.21(5) 3 3_556
Co2 Al4 Ce1 164.38(8) 7_666 .
Co2 Al4 Ce1 87.83(6) 7_665 .
Al2 Al4 Ce1 63.88(6) . .
Al1 Al4 Ce1 124.09(8) 7_665 .
Al3 Al4 Ce1 138.54(5) 7_665 .
Al9 Al4 Ce1 116.26(9) 3_556 .
Al9 Al4 Ce1 64.80(4) 3 .
Al1 Al4 Ce1 60.79(6) 3_556 .
Co2 Al4 Ce1 87.83(6) 7_666 1_556
Co2 Al4 Ce1 164.38(8) 7_665 1_556
Al2 Al4 Ce1 63.88(6) . 1_556
Al1 Al4 Ce1 124.09(8) 7_665 1_556
Al3 Al4 Ce1 138.54(5) 7_665 1_556
Al9 Al4 Ce1 64.80(4) 3_556 1_556
Al9 Al4 Ce1 116.26(9) 3 1_556
Al1 Al4 Ce1 60.79(6) 3_556 1_556
Ce1 Al4 Ce1 77.79(8) . 1_556
Co1 Al5 Ni1 0.00(4) 3 3
Co1 Al5 Co1 102.94(10) 3 3_556
Ni1 Al5 Co1 102.94(10) 3 3_556
Co1 Al5 Ni1 102.94(10) 3 3_556
Ni1 Al5 Ni1 102.94(10) 3 3_556
Co1 Al5 Ni1 0.00(4) 3_556 3_556
Co1 Al5 Al8 56.29(5) 3 3_556
Ni1 Al5 Al8 56.29(5) 3 3_556
Co1 Al5 Al8 56.29(5) 3_556 3_556
Ni1 Al5 Al8 56.29(5) 3_556 3_556
Co1 Al5 Al3 112.44(7) 3 .
Ni1 Al5 Al3 112.44(7) 3 .
Co1 Al5 Al3 112.44(7) 3_556 .
Ni1 Al5 Al3 112.44(7) 3_556 .
Al8 Al5 Al3 100.79(9) 3_556 .
Co1 Al5 Al2 58.05(6) 3 3_556
Ni1 Al5 Al2 58.05(6) 3 3_556
Co1 Al5 Al2 58.05(6) 3_556 3_556
Ni1 Al5 Al2 58.05(6) 3_556 3_556
Al8 Al5 Al2 58.85(7) 3_556 3_556
Al3 Al5 Al2 159.65(12) . 3_556
Co1 Al5 Al6 117.41(10) 3 3_556
Ni1 Al5 Al6 117.41(10) 3 3_556
Co1 Al5 Al6 50.37(6) 3_556 3_556
Ni1 Al5 Al6 50.37(6) 3_556 3_556
Al8 Al5 Al6 100.95(8) 3_556 3_556
Al3 Al5 Al6 129.70(7) . 3_556
Al2 Al5 Al6 60.70(7) 3_556 3_556
Co1 Al5 Al6 50.37(6) 3 3
Ni1 Al5 Al6 50.37(6) 3 3
Co1 Al5 Al6 117.41(10) 3_556 3
Ni1 Al5 Al6 117.41(10) 3_556 3
Al8 Al5 Al6 100.95(8) 3_556 3
Al3 Al5 Al6 129.70(7) . 3
Al2 Al5 Al6 60.70(7) 3_556 3
Al6 Al5 Al6 89.15(11) 3_556 3
Co1 Al5 Al1 108.98(7) 3 3_556
Ni1 Al5 Al1 108.98(7) 3 3_556
Co1 Al5 Al1 108.98(7) 3_556 3_556
Ni1 Al5 Al1 108.98(7) 3_556 3_556
Al8 Al5 Al1 148.47(10) 3_556 3_556
Al3 Al5 Al1 110.73(11) . 3_556
Al2 Al5 Al1 89.62(10) 3_556 3_556
Al6 Al5 Al1 58.61(7) 3_556 3_556
Al6 Al5 Al1 58.61(7) 3 3_556
Co1 Al5 Ce1 88.89(6) 3 .
Ni1 Al5 Ce1 88.89(6) 3 .
Co1 Al5 Ce1 167.55(7) 3_556 .
Ni1 Al5 Ce1 167.55(7) 3_556 .
Al8 Al5 Ce1 135.67(5) 3_556 .
Al3 Al5 Ce1 65.35(6) . .
Al2 Al5 Ce1 128.08(6) 3_556 .
Al6 Al5 Ce1 120.58(9) 3_556 .
Al6 Al5 Ce1 67.37(6) 3 .
Al1 Al5 Ce1 62.67(6) 3_556 .
Co1 Al5 Ce1 167.55(7) 3 1_556
Ni1 Al5 Ce1 167.55(7) 3 1_556
Co1 Al5 Ce1 88.89(6) 3_556 1_556
Ni1 Al5 Ce1 88.89(6) 3_556 1_556
Al8 Al5 Ce1 135.67(5) 3_556 1_556
Al3 Al5 Ce1 65.35(6) . 1_556
Al2 Al5 Ce1 128.08(6) 3_556 1_556
Al6 Al5 Ce1 67.37(6) 3_556 1_556
Al6 Al5 Ce1 120.58(9) 3 1_556
Al1 Al5 Ce1 62.67(6) 3_556 1_556
Ce1 Al5 Ce1 79.07(8) . 1_556
Ni1 Al6 Co2 177.93(13) . .
Ni1 Al6 Al1 118.86(8) . 1_554
Co2 Al6 Al1 59.97(7) . 1_554
Ni1 Al6 Al1 118.86(8) . .
Co2 Al6 Al1 59.97(7) . .
Al1 Al6 Al1 91.69(11) 1_554 .
Ni1 Al6 Al2 58.92(7) . .
Co2 Al6 Al2 122.22(8) . .
Al1 Al6 Al2 177.56(12) 1_554 .
Al1 Al6 Al2 88.75(8) . .
Ni1 Al6 Al2 58.92(7) . 1_554
Co2 Al6 Al2 122.22(8) . 1_554
Al1 Al6 Al2 88.75(8) 1_554 1_554
Al1 Al6 Al2 177.56(12) . 1_554
Al2 Al6 Al2 90.71(11) . 1_554
Ni1 Al6 Al5 58.24(6) . 3_455
Co2 Al6 Al5 120.58(8) . 3_455
Al1 Al6 Al5 60.63(8) 1_554 3_455
Al1 Al6 Al5 121.10(11) . 3_455
Al2 Al6 Al5 117.15(10) . 3_455
Al2 Al6 Al5 57.16(7) 1_554 3_455
Ni1 Al6 Al5 58.24(6) . 3_456
Co2 Al6 Al5 120.58(8) . 3_456
Al1 Al6 Al5 121.11(11) 1_554 3_456
Al1 Al6 Al5 60.63(8) . 3_456
Al2 Al6 Al5 57.16(7) . 3_456
Al2 Al6 Al5 117.15(11) 1_554 3_456
Al5 Al6 Al5 89.15(11) 3_455 3_456
Ni1 Al6 Al3 125.02(7) . .
Co2 Al6 Al3 56.11(6) . .
Al1 Al6 Al3 116.07(10) 1_554 .
Al1 Al6 Al3 56.41(7) . .
Al2 Al6 Al3 66.12(7) . .
Al2 Al6 Al3 125.42(11) 1_554 .
Al5 Al6 Al3 176.34(11) 3_455 .
Al5 Al6 Al3 91.54(7) 3_456 .
Ni1 Al6 Al3 125.02(7) . 1_554
Co2 Al6 Al3 56.11(6) . 1_554
Al1 Al6 Al3 56.41(7) 1_554 1_554
Al1 Al6 Al3 116.07(10) . 1_554
Al2 Al6 Al3 125.42(11) . 1_554
Al2 Al6 Al3 66.12(7) 1_554 1_554
Al5 Al6 Al3 91.54(7) 3_455 1_554
Al5 Al6 Al3 176.34(11) 3_456 1_554
Al3 Al6 Al3 87.55(11) . 1_554
Ni1 Al6 Ce1 91.98(8) . .
Co2 Al6 Ce1 90.08(8) . .
Al1 Al6 Ce1 119.03(7) 1_554 .
Al1 Al6 Ce1 119.03(7) . .
Al2 Al6 Ce1 62.70(7) . .
Al2 Al6 Ce1 62.70(7) 1_554 .
Al5 Al6 Ce1 119.86(7) 3_455 .
Al5 Al6 Ce1 119.86(7) 3_456 .
Al3 Al6 Ce1 62.75(7) . .
Al3 Al6 Ce1 62.75(7) 1_554 .
Co2 Al7 Co1 145.79(11) . 7_655
Co2 Al7 Ni1 145.79(11) . 7_655
Co1 Al7 Ni1 0.00(5) 7_655 7_655
Co2 Al7 Ni1 145.82(10) . 3
Co1 Al7 Ni1 68.39(7) 7_655 3
Ni1 Al7 Ni1 68.39(7) 7_655 3
Co2 Al7 Co1 145.82(10) . 3
Co1 Al7 Co1 68.39(7) 7_655 3
Ni1 Al7 Co1 68.39(7) 7_655 3
Ni1 Al7 Co1 0.00(4) 3 3
Co2 Al7 Al8 136.20(4) . 3_556
Co1 Al7 Al8 53.34(5) 7_655 3_556
Ni1 Al7 Al8 53.34(5) 7_655 3_556
Ni1 Al7 Al8 53.35(5) 3 3_556
Co1 Al7 Al8 53.35(5) 3 3_556
Co2 Al7 Al8 136.20(4) . 3
Co1 Al7 Al8 53.34(5) 7_655 3
Ni1 Al7 Al8 53.34(5) 7_655 3
Ni1 Al7 Al8 53.35(5) 3 3
Co1 Al7 Al8 53.35(5) 3 3
Al8 Al7 Al8 87.60(9) 3_556 3
Ni1 Al8 Co1 180.0 . 5_566
Ni1 Al8 Ni1 180.0 . 5_566
Co1 Al8 Ni1 0.00(5) 5_566 5_566
Ni1 Al8 Co1 70.64(7) . 5_565
Co1 Al8 Co1 109.36(7) 5_566 5_565
Ni1 Al8 Co1 109.36(7) 5_566 5_565
Ni1 Al8 Ni1 70.64(7) . 5_565
Co1 Al8 Ni1 109.36(7) 5_566 5_565
Ni1 Al8 Ni1 109.36(7) 5_566 5_565
Co1 Al8 Ni1 0.00(6) 5_565 5_565
Ni1 Al8 Ni1 109.36(7) . 1_556
Co1 Al8 Ni1 70.64(7) 5_566 1_556
Ni1 Al8 Ni1 70.64(7) 5_566 1_556
Co1 Al8 Ni1 180.0 5_565 1_556
Ni1 Al8 Ni1 180.0 5_565 1_556
Ni1 Al8 Co1 109.36(7) . 1_556
Co1 Al8 Co1 70.64(7) 5_566 1_556
Ni1 Al8 Co1 70.64(7) 5_566 1_556
Co1 Al8 Co1 180.0 5_565 1_556
Ni1 Al8 Co1 180.0 5_565 1_556
Ni1 Al8 Co1 0.00(6) 1_556 1_556
Ni1 Al8 Al2 60.37(4) . .
Co1 Al8 Al2 119.63(4) 5_566 .
Ni1 Al8 Al2 119.63(4) 5_566 .
Co1 Al8 Al2 119.63(4) 5_565 .
Ni1 Al8 Al2 119.63(4) 5_565 .
Ni1 Al8 Al2 60.37(4) 1_556 .
Co1 Al8 Al2 60.37(4) 1_556 .
Ni1 Al8 Al2 119.63(4) . 5_566
Co1 Al8 Al2 60.37(4) 5_566 5_566
Ni1 Al8 Al2 60.37(4) 5_566 5_566
Co1 Al8 Al2 60.37(4) 5_565 5_566
Ni1 Al8 Al2 60.37(4) 5_565 5_566
Ni1 Al8 Al2 119.63(4) 1_556 5_566
Co1 Al8 Al2 119.63(4) 1_556 5_566
Al2 Al8 Al2 180.0 . 5_566
Ni1 Al8 Al5 119.82(4) . 7_665
Co1 Al8 Al5 60.18(4) 5_566 7_665
Ni1 Al8 Al5 60.18(4) 5_566 7_665
Co1 Al8 Al5 60.18(4) 5_565 7_665
Ni1 Al8 Al5 60.18(4) 5_565 7_665
Ni1 Al8 Al5 119.82(4) 1_556 7_665
Co1 Al8 Al5 119.82(4) 1_556 7_665
Al2 Al8 Al5 118.08(7) . 7_665
Al2 Al8 Al5 61.92(7) 5_566 7_665
Ni1 Al8 Al5 60.18(4) . 3_456
Co1 Al8 Al5 119.82(4) 5_566 3_456
Ni1 Al8 Al5 119.82(4) 5_566 3_456
Co1 Al8 Al5 119.82(4) 5_565 3_456
Ni1 Al8 Al5 119.82(4) 5_565 3_456
Ni1 Al8 Al5 60.18(4) 1_556 3_456
Co1 Al8 Al5 60.18(4) 1_556 3_456
Al2 Al8 Al5 61.92(7) . 3_456
Al2 Al8 Al5 118.08(7) 5_566 3_456
Al5 Al8 Al5 180.0 7_665 3_456
Co2 Al9 Co2 180.0 . 5
Co2 Al9 Al1 119.64(5) . 5
Co2 Al9 Al1 60.36(5) 5 5
Co2 Al9 Al1 119.64(5) . 5_556
Co2 Al9 Al1 60.36(5) 5 5_556
Al1 Al9 Al1 92.55(9) 5 5_556
Co2 Al9 Al1 60.36(5) . 1_554
Co2 Al9 Al1 119.64(5) 5 1_554
Al1 Al9 Al1 87.45(9) 5 1_554
Al1 Al9 Al1 180.00(7) 5_556 1_554
Co2 Al9 Al1 60.36(5) . .
Co2 Al9 Al1 119.64(5) 5 .
Al1 Al9 Al1 180.0 5 .
Al1 Al9 Al1 87.45(9) 5_556 .
Al1 Al9 Al1 92.55(9) 1_554 .
Co2 Al9 Al4 56.16(5) . 7_655
Co2 Al9 Al4 123.84(5) 5 7_655
Al1 Al9 Al4 123.55(7) 5 7_655
Al1 Al9 Al4 63.48(7) 5_556 7_655
Al1 Al9 Al4 116.52(7) 1_554 7_655
Al1 Al9 Al4 56.45(7) . 7_655
Co2 Al9 Al4 123.84(5) . 3_455
Co2 Al9 Al4 56.16(5) 5 3_455
Al1 Al9 Al4 56.45(7) 5 3_455
Al1 Al9 Al4 116.52(7) 5_556 3_455
Al1 Al9 Al4 63.48(7) 1_554 3_455
Al1 Al9 Al4 123.55(7) . 3_455
Al4 Al9 Al4 180.0 7_655 3_455
Co2 Al9 Al4 56.16(5) . 7_654
Co2 Al9 Al4 123.84(5) 5 7_654
Al1 Al9 Al4 63.48(7) 5 7_654
Al1 Al9 Al4 123.55(7) 5_556 7_654
Al1 Al9 Al4 56.45(7) 1_554 7_654
Al1 Al9 Al4 116.52(7) . 7_654
Al4 Al9 Al4 87.47(9) 7_655 7_654
Al4 Al9 Al4 92.53(9) 3_455 7_654
Co2 Al9 Al4 123.84(5) . 3_456
Co2 Al9 Al4 56.16(5) 5 3_456
Al1 Al9 Al4 116.52(7) 5 3_456
Al1 Al9 Al4 56.45(7) 5_556 3_456
Al1 Al9 Al4 123.55(7) 1_554 3_456
Al1 Al9 Al4 63.48(7) . 3_456
Al4 Al9 Al4 92.53(9) 7_655 3_456
Al4 Al9 Al4 87.47(9) 3_455 3_456
Al4 Al9 Al4 180.00(12) 7_654 3_456
Co2 Al9 Ce1 91.05(3) . 3_455
Co2 Al9 Ce1 88.95(3) 5 3_455
Al1 Al9 Ce1 118.28(5) 5 3_455
Al1 Al9 Ce1 118.28(5) 5_556 3_455
Al1 Al9 Ce1 61.72(5) 1_554 3_455
Al1 Al9 Ce1 61.72(5) . 3_455
Al4 Al9 Ce1 118.07(4) 7_655 3_455
Al4 Al9 Ce1 61.93(4) 3_455 3_455
Al4 Al9 Ce1 118.07(4) 7_654 3_455
Al4 Al9 Ce1 61.93(4) 3_456 3_455
Co2 Al9 Ce1 88.95(3) . 7_655
Co2 Al9 Ce1 91.05(3) 5 7_655
Al1 Al9 Ce1 61.72(5) 5 7_655
Al1 Al9 Ce1 61.72(5) 5_556 7_655
Al1 Al9 Ce1 118.28(5) 1_554 7_655
Al1 Al9 Ce1 118.28(5) . 7_655
Al4 Al9 Ce1 61.93(4) 7_655 7_655
Al4 Al9 Ce1 118.07(4) 3_455 7_655
Al4 Al9 Ce1 61.93(4) 7_654 7_655
Al4 Al9 Ce1 118.07(4) 3_456 7_655
Ce1 Al9 Ce1 180.000(13) 3_455 7_655
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Ce1 Al1 3.142(2) 3_556
Ce1 Al1 3.142(2) 3
Ce1 Al2 3.147(2) 1_554
Ce1 Al2 3.147(2) .
Ce1 Al5 3.160(2) 1_554
Ce1 Al5 3.160(2) .
Ce1 Al3 3.184(2) 1_554
Ce1 Al3 3.184(2) .
Ce1 Al6 3.191(2) .
Ce1 Al4 3.203(2) 1_554
Ce1 Al4 3.204(2) .
Ce1 Al9 3.2849(7) 3
Ni1 Al6 2.329(3) .
Ni1 Al8 2.4653(17) .
Ni1 Al8 2.4653(17) 1_554
Ni1 Al7 2.537(3) 7_665
Ni1 Al7 2.535(3) 3_455
Ni1 Al5 2.571(2) 3_455
Ni1 Al5 2.571(2) 3_456
Ni1 Al2 2.573(2) .
Ni1 Al2 2.573(2) 1_554
Ni1 Co1 2.851(2) 5_565
Ni1 Ni1 2.851(2) 5_565
Co2 Al9 2.3480(11) .
Co2 Al6 2.355(3) .
Co2 Al7 2.464(3) .
Co2 Al3 2.523(2) .
Co2 Al3 2.523(2) 1_554
Co2 Al4 2.524(2) 7_654
Co2 Al4 2.524(2) 7_655
Co2 Al1 2.607(2) 1_554
Co2 Al1 2.607(2) .
Al1 Co2 2.607(2) 1_556
Al1 Al4 2.695(3) 7_655
Al1 Al3 2.701(3) .
Al1 Al9 2.783(2) .
Al1 Al9 2.783(2) 1_556
Al1 Al6 2.804(3) .
Al1 Al6 2.804(3) 1_556
Al1 Al5 2.862(3) 3_456
Al1 Al4 2.997(3) 3_456
Al1 Ce1 3.142(2) 3_455
Al1 Ce1 3.142(2) 3_456
Al2 Co1 2.573(2) 1_556
Al2 Ni1 2.573(2) 1_556
Al2 Al8 2.642(2) .
Al2 Al4 2.686(3) .
Al2 Al5 2.724(3) 3_456
Al2 Al6 2.827(3) 1_556
Al2 Al6 2.827(3) .
Al2 Ce1 3.147(2) 1_556
Al3 Co2 2.523(2) 1_556
Al3 Al5 2.693(3) .
Al3 Al4 2.741(3) 7_655
Al3 Al6 2.907(3) 1_556
Al3 Al6 2.907(3) .
Al3 Ce1 3.184(2) 1_556
Al4 Co2 2.524(2) 7_666
Al4 Co2 2.524(2) 7_665
Al4 Al1 2.695(3) 7_665
Al4 Al3 2.741(3) 7_665
Al4 Al9 2.910(2) 3_556
Al4 Al9 2.910(2) 3
Al4 Al1 2.997(3) 3_556
Al4 Ce1 3.204(2) 1_556
Al5 Co1 2.571(2) 3
Al5 Ni1 2.571(2) 3
Al5 Co1 2.571(2) 3_556
Al5 Ni1 2.571(2) 3_556
Al5 Al8 2.653(2) 3_556
Al5 Al2 2.724(3) 3_556
Al5 Al6 2.866(3) 3_556
Al5 Al6 2.866(3) 3
Al5 Al1 2.862(3) 3_556
Al5 Ce1 3.160(2) 1_556
Al6 Al1 2.804(3) 1_554
Al6 Al2 2.827(3) 1_554
Al6 Al5 2.866(3) 3_455
Al6 Al5 2.866(3) 3_456
Al6 Al3 2.907(3) 1_554
Al7 Co1 2.537(3) 7_655
Al7 Ni1 2.537(3) 7_655
Al7 Ni1 2.535(3) 3
Al7 Co1 2.535(3) 3
Al7 Al8 2.906(2) 3_556
Al7 Al8 2.906(2) 3
Al8 Co1 2.4653(17) 5_566
Al8 Ni1 2.4653(17) 5_566
Al8 Co1 2.4653(17) 5_565
Al8 Ni1 2.4653(17) 5_565
Al8 Ni1 2.4653(17) 1_556
Al8 Co1 2.4653(17) 1_556
Al8 Al2 2.642(2) 5_566
Al8 Al5 2.653(2) 7_665
Al8 Al5 2.653(2) 3_456
Al9 Co2 2.3480(11) 5
Al9 Al1 2.783(2) 5
Al9 Al1 2.783(2) 5_556
Al9 Al1 2.783(2) 1_554
Al9 Al4 2.910(2) 7_655
Al9 Al4 2.910(2) 3_455
Al9 Al4 2.910(2) 7_654
Al9 Al4 2.910(2) 3_456
Al9 Ce1 3.2849(7) 3_455
Al9 Ce1 3.2849(7) 7_655
